Relationships between longitudinal wave velocity (VL), transverse wave velocity (VS), ratio of sand velocities (VS/VL), ceramic bulk density (ρ), and planar coupling factor (kp) in lead-free and lead-containing ceramics.
This chapter consists of two parts; the first part describes “how can high piezoelectricity be realized from measuring acoustic wave velocities?” That is, the measurement of sound velocities resulted in an effective tool for researching and developing piezoelectric materials, and, furthermore, it was possible to design the material compositions of lead-free piezoelectric ceramics as well as lead-containing ceramics. The second part describes the “effects of firing and DC poling treatments on elastic constants measured from acoustic wave velocities in barium titanate piezoelectric ceramics”. Namely, it could be applied to manufacturing processes such as firing and DC poling treatments in piezoelectric ceramics, which is accompanied with densification of ceramics and ferroelectric domain aligment, respectively. It is clarified through the two parts that the evaluation of elastic constants leads to the origin of piezoelectricity in piezoelectric ceramics.
- origin of piezoelectricity
- piezoelectric ceramics
- acoustic wave velocities
- elastic constants
- domain alignment
1.1. How can high piezoelectricity be realized from measuring acoustic wave velocities?
Lead-free piezoelectric ceramics have been studied by many researchers [1-4], because of replacing Pb(Zr, Ti)O3 (PZT) ceramics. There are three major chemical compositions: alkali niobate , alkali bismuth titanate , and barium titanate . While relatively high piezoelectricity is realized in alkali niobate (the piezoelectric strain d33 constant is 307 pC/N in 0.95(Na, K, Li, Ba)(Nb0.9Ta0.1)O3-0.05SrZrO3 with a small amount of MnO [5, 8]) and barium titanate, low piezoelectricity with low dielectric constant and high mechanical quality factor is obtained in alkali bismuth titanate.
Improving the piezoelectricity in lead-free ceramics, a study on Young’s modulus (Y) vs. piezoelectricity is important how to realize higher piezoelectricity in piezoelectric materials. We have already reported Y in PZT [9-13], PbTiO3 (PT) , BaTiO3 (BT) , alkali niobate ceramics composed of (Na, K, Li, Ba)(Nb0.9Ta0.1)O3-SrZrO3 (SZ) [5, 8] and in a relaxor single crystal of Pb[(Zn1/3Nb2/3)0.91Ti0.09]O3 (PZNT) [15-17] by measuring the impedance responses in various kinds of piezoelectric resonators. Figure 1 shows the relationships between Y and electromechanical coupling factors of transverse mode (k31) and longitudinal mode (k33) in piezoelectric materials. From these figures, it is clarified that the decrease in Y increased the piezoelectricity such as k31 and k33, because materials with lower Y were easy to deform by DC poling field. Therefore, it is said that the measurement of Y was important to obtain high piezoelectricity.
Recently, we developed a novel method to easily measure acoustic wave velocities suitable for conventional disk samples with ordinary dimensions (10-20 mm diameter and 0.5-2.0 mm thickness) by an ultrasonic thickness gauge with high-frequency pulse oscillation [18-20]. Therefore, this method was applied to hard and soft PZT [9-13, 21] and lead-free ceramics composed of alkali niobate [5, 8] and alkali bismuth titanate . In this pursuit, we report the acoustic wave velocities in piezoelectric ceramics measured by our developed method and the calculation results of Young’s modulus, Poisson’s ratio, modulus of rigidity and bulk modulus, especially to obtain high piezoelectricity in lead-free ceramics. Furthermore, we propose the design for R&D on piezoelectric materials from a viewpoint of measuring acoustic wave velocities.
1.2. Experimental procedure
The piezoelectric ceramic compositions measured were as follows: 0.05Pb(Sn0.5Sb0.5)O3-(0.95-
DC poling was conducted for 30 minutes at the most suitable poling temperature (TP) depending on the Curie points of the ceramic materials. The DC poling field (E) depended on the coercive fields and the insulation resistance of the piezoelectric ceramics. The DC poling conditions are as follows: E = 3, 000 V/mm and TP = 150 ℃ for SZ; E = 2, 500-3, 000 V/mm and TP = 70 ℃ for KBT and BT; E = 3, 000 V/mm and TP = 80 ℃ for hard and soft PZT; E = 4, 000 V/mm and TP = 80 ℃ for PLT; E = 4, 000 V/mm and TP = 200 ℃ for PT, respectively. Before and after DC poling, the dielectric and piezoelectric properties were measured at room temperature using an LCR meter (HP4263A), a precision impedance analyzer (Agilent 4294A), and a piezo-d33 meter (Academia Sinica ZJ-3D). Furthermore, the acoustic wave velocities were measured using an ultrasonic precision thickness gauge (Olympus 35DL), which has PZT transducers with 30 MHz for longitudinal wave (VL) generation and 20 MHz for transverse wave (VS) generation . The acoustic wave velocities were evaluated on the basis of the propagation time between the second-pulse echoes in the thickness of ceramic disks parallel to the poling field with dimensions of 14 mm diameter and 0.5-1.5 mm thickness [18-20]. The sample thickness was measured using a precision micrometer (Mitutoyo MDE-25PJ). The number (
where ρ is the bulk density of the ceramic disks. Figure 2 shows the relationships between the ratio of sound velocities (VS/VL), the elastic constants, and dielectric and piezoelectric constants.
1.3. Results and discussion
1.3.1. Dependence of planar coupling factor on elastic constant
Figure 3 shows the relationships between longitudinal (VL) and transverse (VS) wave velocities, Young’s modulus (Y), Poisson’s ratio (σ), modulus of rigidity (G), and bulk modulus (K) vs. planar coupling factors (kp) of disk in (1-
In comparison with the values of before poling (the kp was made use of the values after poling; marks and dash lines in Figure 3), VL, σ, and K increase and VS, Y, and G decrease after poling because of ferroelectric domain alignment. In addition, while the correlation coefficients in the kp vs. Y, σ, and G were almost independent of poling treatment, the coefficients in the kp vs. K after poling increases from 0.49 to 0.74. It is thought that the increase in K is significant to realize piezoelectricity as mentioned below.
Figure 4 shows the relationships between kp vs. changes (Δ) in longitudinal (VL) and transverse wave velocities (VS) [ΔVL/ΔVS], and changes in Young’s modulus (Y), Poisson’s ratio (σ), bulk modulus (K), and rigidity (G) [ΔY/Δσ/ΔK/ΔG] before and after DC poling in soft and hard PZT, PbTiO3 (PT/PLT), alkali niobate (SZ), and alkali bismuth titanate (KBT/ BT). Higher kp was realized in the regions of large +ΔVL and +ΔK, and larger -ΔVS, -ΔY, and -ΔG. There were thresholds regarding kp vs. ΔVS, ΔY, and ΔG around -5%, -7%, and -10%, respectively. On the other hand, there were no thresholds in the cases of kp vs. ΔVL and ΔK, especially Δσ. As there were kp peaks regarding Δσ in hard and soft PZT ceramics and kp maximum in alkali niobate (SZ) ceramics, the compositions in kp peaks and kp maximum correspond to a morphotropic phase boundary (MPB) in PZT  and to take lowest value of VS/VL in SZ (see the following Figure 10). We believe that the origin of piezoelectricity in piezoelectric ceramics was due to large change in VS (-ΔVS) while applying DC poling field parallel to the thickness of disks. Therefore, the larger changes in VS (-ΔVS) correspond to larger changes in Y (-ΔY) and G (-ΔG). These phenomena mean that the origin of high piezoelectricity was due to the mechanical softness of the materials under compress stress (large +ΔVL and +ΔK). In addition, the realization of high piezoelectricity is easy deformation by DC poling field in diameter (large -ΔG) as well in thickness (large -ΔY).
Figure 5 shows schematic charts between domain alignment and the changes in Y, σ, G, and K after DC poling. Comparing domain alignment before poling to the alignment after poling, same charges (+ or -) are generated and gathered in the regions of each ends by opposite charge due to DC poling field, namely orientation polarization which occurs by domain alignment. The orientation polarization acts by reducing of Y and G by repulsion to each other because there are same charges in domain alignment. The enhancing σ and K can be explained by the same phenomena. Therefore, it can be said that higher domain alignment leads to large changes in Y, G, and K. However, large change in σ (+Δσ in Figure 4) does not lead to higher domain alignment since σ value is decided by the combinations of Y (G) and K after poling.
1.3.2. Design for research and development on lead-free piezoelectric ceramics
Figure 6 shows the relationship between VS/VL vs. kp. The kp linearly increased with decreasing VS/VL in lead-free ceramics as well as lead-containing ceramics such as PZT, PLT, and PT. Furthermore, it was confirmed that VS/VL was an effective figure to evaluate both the elastic constants and the piezoelectric constants.
When we research and develop new piezoelectric ceramics with high piezoelectricity in lead-free ceramics, we must need a new concept different from the conventional research looking for chemical compositions such as MPB . From the equations (1)-(4) and the change in VL and VS before and after poling as mentioned previously (Figure 4), we focused on the ceramic bulk density (ρ). Figure 7 shows the relationship VS/VL vs. ρ: ρ of lead-containing ceramics (PZT, PLT, and PT) was independent of VS/VL. However, in lead-free ceramics (SZ, KBT, and BT) ρ decreased with decreasing VS/VL. In the case of ρ vs. kp in Figure 8, although kp in lead-containing ceramics (PZT, PLT, and PT) is independent of VS/VL, kp in lead-free ceramics (SZ, KBT, and BT) increased with decreasing ρ. From the above results, we came to an important concept to obtain lead-free ceramics with high piezoelectricity, namely the R&D on lead-free ceramics with lower bulk density. As a result, it confirmed the importance of measuring VL and VS to evaluate the piezoelectricity.
It was said that the direction of the R&D on lead-free piezoelectric ceramics with high piezoelectricity was looking for ceramics with lower bulk density. For example, in perovskite structure, small cations at A and B sites in perovskite structure of ABO3 were selected. In addition, for practical use, the Curie point (Tc) or depolarization temperature must be over 250 ℃. From the two items we will expect the candidates for new lead-free ceramics such as SrTeO3 (ρ = 4.82 g/cm3, Tc = 485 ℃) and YMnO3 (Tc = 640 ℃), in addition to KNbO3 (ρ = 4.62 g/cm3, Tc = 418 ℃) and LiNbO3 (ρ = 4.46 g/cm3, Tc = 1, 210 ℃), respectively [26, 27]. In fact, the bulk density (ρ) of SZ, which possessed the highest kp [5, 8] in lead-free ceramics we investigated, was around 4.6 g/cm3.
1.3.3. Ferroelectricity in almost same ceramic bulk density
In addition to the relationships between VS/VL vs. kp in Table 1, we evaluated the chemical composition dependence of VS/VL in piezoelectric ceramics. Figure 9 shows the composition
We applied this novel method to 0.05Pb(Sn0.5Sb0.5)O3-(0.95-
1.3.4. Relationship between the ratio of transverse wave velocity to longitudinal wave velocity and Poisson’s ratio
Figure 12 shows the relationship between VS/VL vs. σ in solids including piezoelectric ceramics. The equation between σ, VL, and VS is shown in this figure. All of the σ in solids was plotted on a line of the equation. The VS/VL regions of Poisson’s ratio in soft PZT, hard PZT, lead-free and PbTiO3 (PLT and PT) were also shown in this figure. The regions of σ regarding VS/VL increased from PbTiO3, lead-free, hard PZT to soft PZT with increasing piezoelectricity. In addition to higher Poisson’s ratio, it was clarified that higher kp can be realized in lager K as shown in Figure 3. We believe the physical meaning of this behavior toward σ is as follows: increasing mechanical softness (lower Y) in piezoelectric materials, it becomes easy to deform by DC poling field. The σ becomes larger while the materials become softer, and furthermore, the K must become larger in order to transmit effectively from longitudinal deformation (the directions of poling and applying electric field are thickness direction of disk) to transverse deformation (the radial direction of disk). In this study, it was described a road map in piezoelectric ceramics regarding the relationships between longitudinal and transverse wave velocities, Young’s modulus, Poisson’s ratio, modulus of rigidity and bulk modulus to research and develop new piezoelectric ceramic materials, especially lead-free ceramics with high piezoelectricity.
1.4. Conclusions in this part
Longitudinal and transverse wave velocities in PZT, lead titanate, and lead-free ceramics were measured by an ultrasonic precision thickness gauge with high-frequency pulse generation to calculate elastic constants such as Young’s modulus, Poisson’s ratio, and so forth. Since the ceramic bulk density was focused on to improve piezoelectricity in lead-free ceramics, the candidates of lead-free ceramic compositions with high piezoelectricity were proposed. It was confirmed that our evaluation method was an effective tool for R&D on piezoelectric material. Furthermore, the origin of piezoelectricity in piezoelectric ceramics could be explained by the elastic constants before and after DC poling.
2. Effects of firing and DC poling treatments on elastic constants measured from acoustic wave velocities in barium titanate piezoelectric ceramics
Recently, we have developed a method to evaluate elastic constants, such as Young’s modulus and Poisson’s ratio, by measuring longitudinal and transverse wave velocities using an ultrasonic thickness gauge with high-frequency generation in comparison with a conventional method . This method has been confirmed to be useful for measuring ceramic disks with diameters of 10-20 mm and thicknesses of 0.5-2.0 mm. In addition, it has been clarified that this method is suitable for evaluating cases involving (1) firing process analysis, such as the analysis of the effect of lead oxide (PbO) atmosphere during firing on the dielectric and piezoelectric properties of lead zirconate titanate (PZT) ceramics, and the oxygen atmosphere firing of PZT ceramics to realize pore-free ceramics, (2) DC poling process analysis, such as the analysis of the DC poling field dependence in as-fired (before poling) ceramics and relaxor single crystals, and (3) piezoelectric materials research and development (R&D) for lead-free ceramics with high piezoelectricity from the viewpoints of elastic constants [18-20].
In this part, to clarify the effects of firing temperature and DC poling on barium titanate (BT) piezoelectric ceramics, we studied the firing temperature and DC poling dependences on acoustic wave velocities and dielectric and piezoelectric properties of BT ceramics. Here, we report the relationships between firing temperature and DC poling effect vs. acoustic wave velocities, Young’s modulus, Poisson’s ratio, modulus of rigidity, and bulk modulus.
2.2. Experimental procedure
The BT raw materials in this study were utilized for two types of powder particle with high purities above 99.95% and average particle sizes of 0.2 μm (abbreviated to BT02) and 0.5 μm (BT05) (Sakai Chemical Industry). After firing at 1, 300-1, 350 ℃ for BT02 and at 1, 300-1, 360 ℃ for BT05 for 2 h, the bulk density (ρ) and microstructure of the obtained ceramic disks were evaluated. DC poling was conducted at a temperature of 60 ℃ and a field of 2.0 kV/mm for 30 min. After DC poling, dielectric and piezoelectric properties were measured at room temperature using an LCR meter (HP4263A), a precision impedance analyzer (Agilent 4294A), and a piezo-d33 meter (Academia Sinica ZJ-3D). Furthermore, the acoustic wave velocities of the BT ceramics before and after poling were measured using an ultrasonic precision thickness gauge (Olympus 35DL), which has PZT transducers with a frequency of 30 MHz for longitudinal wave generation and a frequency of 20 MHz for transverse wave generation. The acoustic wave velocities were evaluated on the basis of the propagation time between the second-pulse and the third-pulse echoes in the thickness direction parallel to the DC poling field for the ceramic disks with 14 mm diameter and 0.9-1.2 mm thickness [18-20]. The sample thickness was measured using a precision micrometer (Mitutoyo MDE-25PJ). The number (
2.3. Results and discussion
2.3.1. Firing temperature dependence of dielectric and piezoelectric properties
Figures 13(a)-(d) show the relationships between firing temperature (FT) and (a) relative dielectric constant (εr), (b) planar coupling factor (kp) for the radial mode on the disks, (c) frequency constant (fcp), and (d) piezoelectric strain d33 constant in the cases of BT02 and BT05 ceramics before and after DC poling. Although εr decreases with increasing FT, kp, fcp, and d33 with increasing FT; furthermore, there is an optimum FT of 1, 340 ℃ in BT02 for obtaining the highest kp and d33. The differences in the dielectric and piezoelectric properties vs. FT between BT02 and BT05 were due to the ceramic bulk density, as mentioned later (see the following Figure 17), and the powder particle activity during firing because the specific surface areas of BT02 and BT05 powder particles measured by the Brunauer, Emmett, and Teller (BET) method were 9.4 and 2.3 m2/g, respectively.
2.3.2. Effects of firing temperature and DC poling on acoustic wave velocities and elastic constants
Figures 14(a)-(d) show the relationships between FT and (a) longitudinal wave velocity (VL), (b) transverse wave velocity (VS), (c) Young’s modulus (Y), and (d) Poisson’s ratio (σ) in the cases of BT02 and BT05 ceramics. Although VL, VS, and Y before and after DC poling increase with increasing FT, σ after poling is almost independent of FT; furthermore, there is an optimum FT of 1, 340 ℃ in BT02 from the plots of FT vs. VL and Y. The increase in Y with increasing FT indicates the increase in the mechanical hardness of the ceramic disks. By comparing FT vs. VL in Figure 14(a) with FT vs. 2fcp (fcp is shown in Figure 13(c), the dependences of VL and 2fcp on FT were almost the same, because both of them correspond to longitudinal wave velocities, as shown in Figure 15. In addition, we confirmed that VL precisely corresponded to 2fct, which is twice the frequency constant (fct) of the coupling factor (kt) for the thickness mode on the disks measured using the typical impedance vs. frequency response (Figure 15) . Therefore, it is considered that our measurement method using the ultrasonic precision thickness gauge is suitable for evaluating acoustic wave velocities, especially in piezoelectric ceramics.
Figures 16(a)-(b) show the changes in Y (ΔY) and σ (Δσ) during poling, respectively. ΔY decreases with increasing FT, regardless of the types of BT powder particle. This phenomenon indicates that the ceramics become mechanically softer after DC poling. It is considered that such a change is due to the ferroelectric domain () alignment induced by the poling field, such as a change in the configuration from a random orientation () before poling to a directional orientation () after poling [5-7, 9-15]. Δσ abruptly increases from FT of 1, 320 ℃ and shows almost the same tendency as in the case of FT vs. kp in Figure 13(b). By comparing FT vs. kp (Figure 13(b)) with FT vs. Δσ (Fig. 16(b)), a higher kp was obtained in the case of a larger Δσ. The physical meaning of the phenomenon regarding σ was deduced, that is, a larger Δσ was needed to realize a higher kp because of the easy deformation of the bulk perpendicular to the poling field (radial direction in the disks) as well as parallel to the poling field (thickness direction in the disks).
2.3.3. Relationship between ceramic microstructure and elastic constants
Figure 17 shows the FT dependence of the bulk density (ρ) of the ceramic disks. The relative bulk density (ρ/ρ0) became over 94% for both BT02 and BT05 during firing at 1, 340-1, 360 ℃, where ρ0 (6.02 g/cm3) is the theoretical density of BT ceramics . From our previous study on the relationships between kp vs. Y and σ in piezoelectric ceramics, a higher kp was realized at a lower Y and a higher σ [18-20]. However, there is no correspondence between the lower Y (Fig. 14(c)), the higher σ (Fig. 14(d)), the lower kp (Fig. 13(b)), and the lower d33 (Fig. 13(d)) during firing at 1, 300-1, 320 ℃ because of the low relative bulk density of ρ/ρ0 (< 0.94). On the other hand, while Y became almost constant during firing at 1, 340-1, 360 ℃ (Fig. 14(c)), σ before poling decreased with increasing FT (Fig. 14(d)). It was considered that the decrease in σ with increasing FT was due to the increase in the density of coarse grains with average diameters of 50 μm as mentioned later. As FT vs. σ before poling (Fig. 14(d)) shows the same tendency as FT vs. εr (Fig. 13(a)), the εr of which is directly related to ferroelectric domain structures, the σ dependence of FT was considered to be due to the domain structures and anisotropy of coarse grains being different from those of fine grains with average diameters of 1.2 μm. Since the ferroelectric domain size increases with increasing grain size of BT ceramics, the domain density decreases in the case of coarse grains [30-33]. Therefore, the ceramics with coarse grains exhibit a lower εr and a larger crystal anisotropy than the ceramics with fine grains [34-38]. Furthermore, σ decreases with increasing FT because it approaches a behavior similar to that of a BT single crystal, σ of which is 0.29 while σ of the ceramics is 0.31 . In order to evaluate the physical characteristics of ceramic grains, the modulus of rigidity (G) and bulk modulus (K) were calculated by the equations (3) and (4) in Section 1.2. [23, 24]: G and K before poling increase with increasing FT during firing at 1,300-1,360 ℃, as shown in Figures 18(a)-(b), respectively, because the ceramic bulk density is improved in BT ceramics as shown in Figure 17; as a result, G and K are obtained from the equations (3) and (4), as well as Y in Figure 14(c) from equation (1). On the other hand, σ is independent of the ceramic bulk density, as shown in equation (2). Figures 19(a)-(d) show the relationships between ρ/ρ0 vs. Y, σ, G, and K, respectively. Y, G, and K depend on ρ/ρ0 because they are affected by increasing the mechanical strength, especially the hardness of the ceramics, with FT. As mentioned previously regarding Figure 14(d), σ is independent of ρ/ρ0 except when ρ/ρ0 is above 0.94, as shown in Figure 19(b), which corresponds to ceramics with a larger domain size and a lower domain density with coarse grains. G decreased and K increased after poling owing to the domain alignment as shown in Figure 18. In addition, the change in G (ΔG) in BT ceramics during poling linearly decreased with increasing FT, and peaks of the changes in K (ΔK), which correspond to the peaks of Δσ (Figure 16(b)), were obtained at FT of 1340 ℃ in the BT02 ceramics and at FT of 1, 350-1, 360 ℃ in the BT05 ceramics, as shown in Figures 20(a)-(b). Therefore, a higher kp could be realized at FT at the peaks of ΔK and Δσ. Since ceramic grains with a higher K due to domain alignment during DC poling, indicating a high ceramic bulk density for obtaining a higher kp, are difficult to change in terms of their volume while applying external stress, the deformation of grains is practically transferred from the parallel direction to the perpendicular direction toward the direction of the applied stress; as a result, a higher σ is achieved. We believe that the increase in σ (Δσ) as a result of the increase in K (ΔK) indicates fundamental issues regarding the poling of ceramic grains to obtain a higher kp; therefore, the R&D of piezoelectric ceramics with high piezoelectricity must be focused on to realize a lower G and a higher K during DC poling from the viewpoints of elastic constants. From the above-mentioned results, it was considered that the values of FT vs. G and K in BT02 and BT05 ceramics after poling (Figures 18(a)-(b)) correspond to the values of kp vs. FT (Figure 13(b)).
Figure 21(a) shows the FT dependence of microstructures in the BT02 ceramics. With the increase in kp with FT, ceramic grains grew from 1.2 μm (fine grains shown as white parts in the figures) to 50 μm (coarse grains shown as black parts in the figures) in diameter; moreover, the ratio of black parts to whole parts (black parts plus white parts) increased. The border between fine and coarse grains is shown in Figures 21(b)-(c). Furthermore, it was found that the black parts consist of several coarse grains, as shown in Figure 21(b). This phenomenon was almost the same as in the case of the microstructure in the BT05 ceramics. Figure 22 shows the relationship between kp and the area ratio of coarse grains (black parts) measured by image-analyzing software (WinROOF ). In this figure, when the area ratio increases, kp increases because of the increase in the density of coarse grains. Therefore, the coarse grains in the dense ceramic bulk contribute to a higher kp and VL, VS, Y, and σ in the coarse grains correspond to those at FT of 1, 360 ℃ in Figures 14(a)-(d), which almost agree with the values previously reported .
2.3.4. Firing temperature dependence of elastic constants in barium titanate ceramics
Figure 23 shows that the relationships between kp vs. Y, σ, G, and K in BT02 and BT05 ceramics fired at different temperatures were inserted into the relationships between kp vs. Y, σ, G, and K in lead-containing and lead-free piezoelectric ceramics (Figure 3), which were fired at the optimal temperatures for each composition to realize the maximum kp. Higher kp is obtained in the cases of lower Y and G, and furthermore, higher σ and K, which are indicated by yellow arrows in Figure 23. This figure also indicates the firing temperature dependence of the bulk density vs. Y, σ, G, and K in BT02 and BT05 ceramics in Figure 19. kp increases with the increase of Y, G, and K because of the increase in bulk density with increasing firing temperature. On the other hand, σ was independent of kp because σ is an intrinsic material constant. These phenomena are indicated by green arrows in Figure 23. It is predicted the same phenomena regarding the firing temperature and bulk density dependences on kp vs. Y, σ, G, and K in cases of lead-containing and lead-free ceramics.
2.4. Conclusions in this part
The effects of firing temperature and DC poling on the longitudinal and transverse wave velocities in barium titanate ceramics were investigated using an ultrasonic precision thickness gauge with high-frequency pulse generation. The results could explain the relationships between acoustic wave velocities, Young’s modulus, Poisson’s ratio, the modulus of rigidity, and the bulk modulus vs. firing temperature, and the changes in elastic constants during DC poling.
3. Summary of this chapter
Sound velocities were evaluated in ceramic disks composed of lead-containing and lead-free ceramics using an ultrasonic precision thickness gauge with high-frequency pulse generation, and furthermore, dielectric and piezoelectric constants were simultaneously measured utilizing the same disk samples. Calculating elastic constants by using the sound velocities, higher piezoelectricity in ceramics were obtained in lower Young’s modulus and rigidity, and furthermore, higher Poisson’s ratio and bulk modulus. Piezoelectric ceramics with lower Young’s modulus and rigidity caused by ferroelectric domain alignment while DC poling were easy to deform by electric field and external force. In addition to these phenomena, higher bulk modulus needs to realize higher Poisson’s ratio. Lower Young’s modulus means mechanical soft in ceramics; however, higher bulk modulus, which means mechanical hard in ceramics, need to obtain higher piezoelectricity. It was thought that these characteristics run counter to the mechanical characteristics of piezoelectric ceramics; however, it was the origin of piezoelectricity in ceramics.
This work was partially supported by two Grants-in-Aid for Scientific Research C (Nos. 21560340 and 26420282), a Grant from the Strategic Research Foundation Grant-Aided Project for Private Universities 2010-2014 (No. S1001032) from the Ministry of Education, Culture, Sports, Science and Technology, Japan (MEXT), and a Cooperation Research Foundation 2014 between Academy and Industry of Fukuroi City, Shizuoka, Japan.
Saito Y, Takao H, Tani T, Nonoyama T, Takatori K, Homma T, Nagaya T, Nakamura M. Lead-free piezoceramics. Nature 2004;432:84-7.
Yang ZP, Liu B, Wei LL, Hou YT. Structure and electrical properties of (1-x)Bi0.5Na0.5 TiO3-xBi0.5K0.5TiO3 ceramics near morphotropic phase boundary. Mater Res Bull 2008;43:81-9.
Zhao W, Zhou HP, Yan YK, Liu D. Morphotropic phase boundary study of the BNT- BKT lead-free piezoelectric ceramics. Key Eng Mater 2008;368-372:1908-10.
Dai YJ, Pan JS, Zhang XW. Composition range of morphotropic phase boundary and electrical properties of NBT-BT system. Key Eng Mater 2007;336-338:206-9.
Ogawa T, Furukawa M, Tsukada T. Poling field dependence of piezoelectric properties and hysteresis loops of polarization versus electric field in alkali niobate ceramics. Jpn J Appl Phys 2009;48:709KD07-1-5.
Ogawa T, Nishina T, Furukawa M, Tsukada T. Poling field dependence of ferroelectric properties in alkali bismuth titanate lead-free ceramics. Jpn J Appl Phys 2010;49:09MD07-1-4.
Ogawa T. Poling field dependence of ferroelectric properties in barium titanate ceramics. Jpn J Appl Phys 2001;40:5630-3.
Furukawa M, Tsukada T, Tanaka D, Sakamoto N. Alkaline niobate-based lead-free piezoelectric ceramics. Proc 24th Int Japan-Korea Semin Ceramics 2007;339-42.
Ogawa T, Yamada A, Chung YK, Chun DI. Effect of domain structures on electrical properties in tetragonal PZT ceramics. J Korean Phys Soc 1998;32:S724-S726.
Ogawa T, Nakamura K. Poling field dependence of ferroelectric properties and crystal orientation in rhombohedral lead zirconate titanate ceramics. Jpn J Appl Phys 1998;37:5241-5.
Ogawa T, Nakamura K. Effect of domain switching and rotation on dielectric and piezoelectric properties in lead zirconate titanate ceramics. Jpn J Appl Phys 1999;38:5465-9.
Ogawa T. Domain switching and rotation in lead zirconate titanate ceramics by poling fields. Ferroelectrics 2000;240:75-82.
Ogawa T. Domain structure of ferroelectric ceramics. Ceram Int 2000;25:383-90.
Ogawa T. Poling field dependence of crystal orientation and ferroelectric properties in lead titanate ceramics. Jpn J Appl Phys 2000;39:5538-41.
Ogawa T. Poling field dependence of ferroelectric properties in piezoelectric ceramics and single crystal. Ferroelectrics 2002;273:371-6.
Kato R, Ogawa T. Chemical composition dependence of giant piezoelectricity on k31 mode in Pb(Mg1/3Nb2/3)O3-PbTiO3 single crystals. Jpn. J. Appl. Phys. 2006;45:7418-21.
Ogawa T. Giant k31 relaxor single-crystal plate and their applications. In Lallart M. (ed.) Ferroelectrics –Applications–. Rijeka: Intech; 2011, pp.3-34 .
Ogawa T, Nishina T. Acoustic wave velocities measurement on piezoelectric ceramics to evaluate Young’s modulus and Poisson’s ratio for realization of high piezoelectricity. In Nair KM, Priya S. (eds.) Ceramic Transactions, Advances and Applications in Electroceramics II. Hoboken: Wiley; 2012;235:pp.105-12.
Ogawa T, Ishii K, Matsumoto T, Nishina T. Poling field dependence of longitudinal and transverse wave velocities, Young’s modulus, and Poisson’s ratio in piezoelectric ceramics. J Appl Phys 2012;51:09LD03-1-5.
Ogawa T. Acoustic wave velocity measurement on piezoelectric ceramics. In Ebrahimi F. (ed.) Piezoelectric Materials and Devices –Practice and Applications–. Rijeka: Intech; 2013, pp.35-52 .
Ogawa T. Highly functional and high-performance piezoelectric ceramics. Ceramic Bull 1991;70:1042-9.
Olympus Co. Ultrasonic Precision Thickness Gages User’s Manual. Part No. 910-261-EN, Revision H. Waltham: Olympus NDT Inc; 2008.
Mason WP. Piezoelectric Crystals and Their Application to Ultrasonics. Princeton: Nostrand; 1950, p.390.
Philippoff W, Brodnyan J. Preliminary results in measuring dynamic compressibilities. J Appl Phys 1955;26:846.
Jaffe B, Cook WR, Jaffe H. Piezoelectric Ceramics. London: Academic Press; 1971.
Landolt-Bornstein Group III. Condensed Matter, Ferroelectrics and Related Substances. Berlin: Springer; 2001, 36A1.
Landolt-Bornstein Group III. Condensed Matter, Ferroelectrics and Related Substances. Berlin: Springer; 2002, 36A2.
Mason WP. Physical Acoustics. New York: Academic Press; 1964, Part A, p.182.
IEEE Standard. 1988;pp.176-1987.
Salje E. Domain mobilities and elastic instabilities in ferroelastic and co-elastic materials. In Phase Transitions in Ferroelastic and Coelastic Crystals. Cambridge: Cambridge University Press; 1990, p.76.
Arlt G. The influence of microstructure on the properties of ferroelectric ceramics. Ferroelectrics 1990;104:217.
Randall CA, Kim N, Kucera JP, Cao W, Shrout TR. Intrinsic and extrinsic size effects in fine-grained morphotropic-phase-boundary lead zirconate titanate ceramics. J Am Ceram Soc 1988;81:677.
Cao W, Randall CA. Grain size and domain size relations in bulk ceramic ferroelectric materials. J Phys Chem Solids 1996;10:1499.
Arlt G, Hennings D, With GD. Dielectric properties of fine-grained barium titanate ceramics. J Appl Phys 1985;58:1619.
Buessem WR, Cross LE, Goswami AK. Phenomenological theory of high permittivity in fine-grained barium titanate. J Am Ceram Soc 1966;49:33.
Kinoshita K, Yamaji A. Grain-size effects on dielectric properties in barium titanate ceramics. J Appl Phys 1976;47:371.
Arlt G, Peusens H. The dielectric constant of coarse grained BaTiO3 ceramics. Ferroelectrics 1983;48:213.
Demartin M, Damjanovic D. Dependence of the direct piezoelectric effect in coarse and fine grain barium titanate ceramics on dynamic and static pressure. Appl Phys Lett 1996;68:3046.